Biomechanical assessment of freeze-dried allograft
cortical bone plate graft in canine bone defect model
, H.B. Lee1
, K.C. Lee1,2
, M.S. Kim1,2
, C.S. Na3
, N.S. Kim1,2
1College of Veterinary Medicine, Chonbuk National University, Jeonju, Republic of Korea 2BioSafety Research Institute, Chonbuk National University, Jeonju Republic of Korea 3College of Agriculture, Chonbuk National University, Jeonju, Republic of Korea
ABSTRACT: Freeze-dried cortical bone can be used as a biological plate, either alone or in combination with other internal fixation devices, to stabilize fractures. In addition to it conferring mechanical stability, freeze-dried cortical bone may enhance fracture-healing and increase the bone stock. This study examined the effect of a freeze-dried allograft cortical bone plate (FACBP) on the biomechanical properties of an implant site in a canine bone defect model. Twelve adult mongrel dogs (around 4.8 kg) were used. A segmental critical-size defect (5 mm in length) at ulna diaphysis was created using an oscillating saw. The experimental animals were divided into two groups: eight dogs treated with an absorbable bone plate (FACBP) fixed by metal bone screws (Group A) and four dogs treated with a commercial stainless steel bone plate and metal bone screws (Group B). Bone healing was assessed by radiography, Dual-energy x-ray absorptiometry and a three-point bending test. The FACBP incorporated in the host bone produced complete remodeling of the cortical bone. There was no significant difference in the bone mineral density and biomechanical tests between the FACBP application site and normal ulna or a stainless steel bone plate of the ulna. These results suggest that FACBP facilitates recovery from a bone fracture by assisting in the induction of new bone formation in a defected fracture.
Keywords: bone defect model; dual-energy x-ray absorptiometry; absorbable bone plate
There has been increasing interest on bone trans-plants in orthopedic surgery. Bone transtrans-plants can be used to treat fractures, nonunion and osteo-myelitis. Other orthopedic indications include limb lengthening, reconstructive procedures after a tumor resection, arthrodeses and osteointegra-tion of joint replacement prostheses. The clinical use of these techniques extends beyond the field of orthopedics to include periodontal, maxillofa-cial and neurosurgery (Sinibaldi, 1989; Wilson et al., 2005). Although autogenous bone is the gold standard that all alternatives must either meet or exceed, autografts have significant limitations, such as an additional surgical incision, donor site mor-bidity, weakened donor bone sites, an inadequate amount and an inappropriate form (Enneking et al., 1980; Burchardt, 1987; Finkemeier, 2002). These limitations have prompted increasing interest in alternative bone grafts.
The most common allograft is freeze-dried and deep-frozen. Preservation is obtained by either freezing or freeze-drying. Both allow extended storage but reduce the immunogenicity of the graft and may alter its mechanical strength. Allografts are processed and preserved in a variety of ways in order to maintain the osteoinductive and osteoconductive capacity of the material as well as to reduce its im-munogenicity (Burchardt, 1987; Vajaradul, 2000).
Bone density changes secondary to plate applica-tion have been documented using biomechanical testing, photon absorptiometry, direct and morpho-metric caliper measurements, ashing procedures, histological and fluorescence microscopy and mi-croradiography (Faulkner et al., 1991; Freeman et al., 1996; Grier et al., 1996; Millis et al., 1998; Ebbesen et al., 1999; Schneider et al., 2004).
Dual-energy x-ray absorptiometry is the
assessment of the bone mineral status in humans (Theodorou and Theodorou, 2002), and is also the method most commonly used in dogs (Freeman et al., 1996; Grier et al., 1996; Lauten et al., 2001). The technique can be performed quickly and has a low radiation dose but relatively high precision and accuracy (Grampp et al., 1993).
Freeze-dried allograft cortical bone (FDACB) can act as a biological plate, either alone or in combina-tion with other internal fixacombina-tion devices, to stabilize fractures (Chandler and Tigges, 1998; Brady et al., 1999). As well as conferring mechanical stability, FDACB may enhance fracture-healing and increase the bone stock (Malinin et al., 1984; Wilson et al., 2005). Previous reports suggested that cortical al-lografts unite, remodel and mature with the host bone (Haddad and Duncan, 2003). However, the long-term effect of a FDACB graft on the implant site is not known.
This study examined the effect of long term FDACB plate application on the implant site den-sity and strength in dogs. The change in cortical bone density was determined by comparing the strength of the implant site of the ulna with that of a normal contralateral ulna or a stainless steel bone plate of the ulna.
MATERIAL AND METHODS
Animals and experimental design
Twelve healthy adult mongrel dogs, weighing 4–6 kg (4.8 ± 1.1 kg), and aged from 2–6 years (4.1 ± 1.7 years) were used in this study. The basic experimental model consisted of an ulna diaphy-sis transverse defect (5 mm in length), which was created using an oscillating saw under continuous saline irrigation. The experimental animals were divided into two groups. Eight dogs with a trans-verse defect ulna were given an absorbable bone plate treated with FDACB and a metal bone screw (Group A). Four dogs with a transverse defect ulna were treated with a stainless steel bone plate and screws (Group B).
Preparation of freeze-dried allograft cortical bone plate cortical bone was obtained from healthy two year old mongrel dogs weighing 25 kg. The ends of the long bones were cut away using a bone band saw. The midshafts were mechanically scraped clean of soft tissues, including the cartilage, periosteum and bone marrow, and washed in cold Ringer’s lactated
solu-tion. The cortical bone was trimmed to the required size using a metal bone plate as a guide. The bones were dried and washed with deionized water for 1 h at 4°C with stirring performed several times. The bones were defatted in a 1 : 1 ratio of chloroform/methanol at 24°C for seven days and kept in flowing air for 1 h at room temperature to remove the residual chloroform and methanol by evaporation. The defatted bones were washed with deionized water, with stirring, for 2 h at 4°C, and frozen at –80°C. The cortical bone plate was placed in a freeze-drying chamber that had been
pre-cooled to –80°C and a vacuum of 10–2 mtorr was
applied. Complete freeze drying took approximately six days. At that time, the moisture of the bone was approximately 5%. The freeze-dried bone was then double-wrapped in sterilized packs of which one side was paper and the side was plastic film. The materials were sterilized by exposure to EO gas and stored at room temperature until needed.
Prior to surgery, the patients received 25 mg/kg
cephalexin (Methilexin®, Union Korea Pharm,
Korea) intramuscularly for prophylaxis. The experi-mental animals were premedicated with 0.02 mg/kg subcutaneous atropine sulfate (Atropine Sulfate
Daewon®, Dae Won Pharm, Korea), induced with
5 mg/kg intravenous propofol (Anepol IN®, Ha
Na Pharm, Korea) and maintained with enflurane and oxygen. The animals were placed in the lateral recumbency position and all surgical procedures were carried out under sterile conditions. A 5-cm longitudinal skin incision was made at the cra-niolateral aspect of the left ulna. The treatment group was given an absorbable bone plate treated with freeze-dried allograft cortical bone with a metal bone screw. (Figure 1) The control group was stabilized with a metal plate and screws ac-cording to the guidelines of the association for a study of internal fixation (ASLF). The muscle attachment was repaired and the skin was close in layers. The animals were allowed to freely bear weight immediately after surgery, and were al-lowed to eat.
distribution of bone formation at the bone defect. In addition, the alignment of the defect ulna was compared with the contralateral ulna.
The fate of the graft was examined by x-ray imag-ing at 2–4 weeks intervals for 135 weeks. The param-eters examined were new bone formation, union of a defected gap, and absorption of a bone plate.
Dual-energy x-ray absorptiometry
After 135 weeks, the dogs were euthanatized by an intravenous administration of sodium
pento-barbital (Entobar Inj®, Han Lim Pharm, Korea).
Each ulna was dissected from the surrounding soft tissues, with care taken to preserve the bone. The bone mineral density (BMD) and bone min-eral content (BMC) were determined by periphmin-eral dual-energy x-ray absorptiometry (GE lunar PIXI-mus2, GE Healthcare, USA). Quality control and calibration were carried out within 24 h of each scanning period. The ulna was divided into three regions of interest, general ulna shaft, implant re-gion and defect rere-gion. (ROI; Figure 2) The analo-gous ROIs were scanned in the intact contralateral
ulnas. Commercially available software (LUNAR Pixi Mus 1.43, GE Healthcare, USA) was used to
determine the bone mineral density (g/cm2) and
bone mineral content (g).
After x-ray absorptiometry, a Universal testing machine (WL2100C; WITH LAB CO., LTD Korea) was used for the biomechanical tests. The flexure stress of the ulna was determined by breaking the bones by 3-point bending (gap size, 30 mm) with the load being applied at a constant displacement of 15 mm/min to failure. The ulna broke in the defect region (Or midshafts ulna of the intact contralateral limb). The maximum load (N) and stiffness (N/min) were interpreted and calculated from the load-de-flection curve, which was displayed continuously on a computer monitor.
The results are presented as the mean ± SEM. Statistical analysis of the data was carried out by one-way analysis of variance (ANOVA). A com-parison of the BMD, BMC, ultimate load at failure
and stiffness were made using a Student’s t-test.
A P value < 0.05 was considered significant.
Figure 1. A 5 mm bone defect was created in the middle of the ulna and was stabilized with freeze-dried allograft cortical bone plate and metal bone screw
All the dogs tolerated the surgical procedures well, and recovered fully without infection, frac-tures about the fixation or the need for additional surgical procedures. All dogs were able to fully bear weight on the limb.
Gross inspection at 135 weeks
In Group A, complete healing of the defect site was observed in all eight dogs. The defect
site showed complete remodeling as a result of the marked adherence to the recipient bone. In Group B, complete healing of the defect site was observed in all four dogs. The defect site showed complete remodeling and fracture healing.
In both groups, the defect site was stable in all ulnas without evidence of screw loosening. In Group A, the radiographs demonstrated a healed fracture, the FDAB plate incorporated in the host bone and complete remodeling of the cortical bone (Figure 3). In Group B, the radiographs
demon-Table 1. Bone mineral density and bone mineral content of the general ulna shaft, implant region, defect ROI for Group A, Group B, and a normal ulna (mean ± SEM)
Group A Group B Normal ulna
ROI1(genernal ulna shaft)
Bone mineral density(g/cm2) 0.37 ± 0.02 0.40 ± 0.006 0.35 ± 0.02
Bone mineralcontent (g) 1.76 ± 0.2 1.64 ± 0.13 1.51 ± 0.09 ROI2(implant region)
Bone mineral density(g/cm2) 0.42 ± 0.02 0.39 ± 0.04 0.39 ± 0.02
Bone mineralcontent (g) 1.08 ± 0.08 1.09 ± 0.03 0.91 ± 0.07 ROI3(defect region)
Bone mineral density(g/cm2) 0.42 ± 0.03 0.40 ± 0.03 0.39 ± 0.01
Bone mineralcontent (g) 0.23 ± 0.09 0.12 ± 0.03 0.09 ± 0.009
ROI = region of interest, Group A = freeze-dried allograft cortical bone plate, Group B = stainless steel bone plate
Figure 6. Biomechanical strength of the bone defect site at 135 weeks. The stiffness of the ulna in Group A was slightly higher than of the normal ulna and Group B. How-ever, the difference was not statistically significant
Figure 4. Radiographs demonstrating a healed defect site in Group B, with partial new bone formation in the implant site. A, B, C, D show 0, 18, 74, 135 weeks after surgery, respectively
Figure 5. Biomechanical strength of the bone defect site at 135 weeks. The maximum load of the ulna in Group A was slightly higher than of the normal ulna and Group B. However, the difference was not statistically significant
strated a fracture union and complete remodeling of the cortical bone (Figure 4).
Dual-energy x-ray absorptiometry
Table 1 shows the BMD and BMC. BMD and BMC of the FDAB plate applied to the ulna (Group A) were similar to those of the stainless steel bone plate ap-plied the ulna (Group B). There were no significant
differences between the two groups (P > 0.05).
Eight ulnas from Group A and four ulnas from Group B (at 135 weeks) were used for the tree-point bending test. Ten normal ulnas were used
as the control. The maximum load (N) to fracture in Group A, Group B, and the control was 6 420 ± 1 166, 4 210 ± 1 232, and 5 478 ± 727 N, respectively (Figure 5.). The stiffness (N/min) for fracture in Groups A, Group B, and the control was 1 572 ± 158, 1 019 ± 173, and 1 438 ±110 N/min, respec-tively (Figure 6.). The maximum load (N) and stiff-ness (N/min) in Group A was slightly higher than that of the normal ulna but the difference was not statistically significant.
The use of various forms of bone grafts to replace or supplement a diseased portion of the skeleton is common in clinical practice. The successful use of these tissues is dependent on various biological,
Group A Group B Normal ulna Group A Group B Normal ulna 8000
7000 6000 5000 4000 3000 2000 1000 0
2000 1800 1600 1400 1200 1000 800 600 400 200 0
physiological, and biomechanical factors, each of which affects the result of the transplant (Burchardt, 1987; Horowitz and Friedlaender, 1987).
This study showed that the effect of long term FDACB plate application on the host bone was similar to that of the control group. A significant loss of bone minerals (up to 50%) develops in a fractured bone during the first six months after an injury. After fracture healing, some recovery of the lost bone occurs (Finsen and Haave, 1987). It was previously reported that the bone mineral decreased rapidly after fracture, which continued for approximately five months. Towards the end of the first year after injury, there was slow restoration of the mineral content but no return to the initial values in most instances. Although the average maximum loss was approximately 45%, only 25% of the initial bone mineral was missing after one year (Andersson and Nilsson, 1979).
Fracture treatment by internal fixation with metal plates is a common practice. However, the applica-tion of a metal plate to the bone has an adverse effect on the bone remolding process (Akeson et al., 1976; Woo et al., 1976; Slatis et al., 1978). In addition, it does not promote osteogenesis (Anderson, 1965). There are significant biological and biomechanical differences in fracture healing between internal and external fixation (Uhthoff and Finnegan, 1983).
The three regions of interest of the ulna where the FDACB plate was applied canine limb were similar to the normal ulna. The long term FDACB plate site showed complete fracture healing and recovery of the bone defect. This suggests that the bone may, under some circumstances, show a local increase in strength after remodeling.
The main finding of this study was that the stain-less steel bone plate groups showed a mean 35% lower maximum load and a 35% lower stiffness than the FDACB groups. The recorded differences indicate that the defect site gained strength once stabilized internally with the FDACB plate. Malinin et al. (1984) reported that refracturing of the radius fixed with an allograft cortical bone plate required 72.9% of the failure load needed to break a normal paired radius. In contrast, a stainless steel-plated radius required only 44.2% of the control load to refacture at eight weeks. These results correspond to those of an earlier study, which reported that an allograft cortical bone plate site was stronger than a stainless steel bone plate site. However, the allograft cortical bone plate site was weaker than the normal ulna. It is believed that in the previous
study, the fracture site had not healed, remodeled and united completely with the host bone. In ad-dition, there was a difference in the observation period compared with the present study. In this study, there was complete healing of the defect site and incorporation in the host bone.
A stainless steel bone plate site creates compres-sion at the interface between the bone cortex and the plate (Moyen et al., 1978; Jain et al., 1997). Local ischemia leads to cortical necrosis with increased haversian remodeling as well as early bone porosis to reestablish the cortical circulation. The produc-tion of newly formed lamellar bone normally occurs within 20 weeks after plate application (Perren et al., 1988).
There is a dynamic change in the allograft bio-mechanics during the incorporation and remod-eling process. The biomechanical response to an allograft onlay strut has been well documented in a canine model (Kreuz et al., 1951; Emerson et al., 1992). The bone-plate allograft augmented the strength in the host bone and promoted healing of the fracture site (Malinin et al., 1984; Zhou et al., 2005a,b). After a 135 week follow-up, there was complete maturation and remodeling in the im-plant site. This study showed host bone fracture healing, anatomical alignment, union and incor-poration in the host bone.
The freeze-dried allograft cortical bone plate united with the fractured bone by incorporating with the host bone, showing complete remodeling without complications. This material can be used clinically as an absorbable internal fixation mate-rial, and can assist in healing by inducing new bone formation in a large defect fracture.
Akeson W.H., Woo S.L., Rutherford L., Coutts R.D., Gonsalves M., Amiel D. (1976): The effects of rigidity of internal fixation plates on long bone remodeling. A biomechanical and quantitative histological study. Acta Orthopaedica Scandinavica,47, 241–249. Anderson L.D. (1965): Treatment of ununited fractures
of the long bones; compression plate fixation and the effect of different types of internal fixation on fracture Healing. The Journal of Bone and Joint Surgery. Amer-ican Volume, 47, 191–208.
Brady O.H., Garbuz, D.S., Masri B.A., Duncan C.P. (1999): The treatment of periprosthetic fractures of the femur using cortical onlay allograft struts. The Orthopedic Clinics of North America, 30, 249–257. Burchardt H. (1987): Biology of bone transplantation.
The Orthopedic Clinics of North America, 18, 187– 196.
Chandler H.P., Tigges R.G. (1998): The role of allografts in the treatment of periprosthetic femoral fractures. Instructional Course Lectures,47, 257–264.
Ebbesen E.N., Thomsen J.S., Beck-Nielsen H., Nepper-Rasmussen H.J., Mosekilde L. (1999): Lumbar vertebral body compressive strength evaluated by dual-energy X-ray absorptiometry, quantitative computed tomog-raphy, and ashing. Bone, 25, 713–724.
Emerson R.H., Malinin T.I., Cuellar A.D., Head W.C., Peters P.C. (1992): Cortical strut allografts in the re-construction of the femur in revision total hip arthro-plasty. A basic science and clinical study. Clinical Orthopaedics and Related Research, 35–44.
Enneking W.F., Eady J.L., Burchardt H. (1980): Autog-enous cortical bone grafts in the reconstruction of segmental skeletal defects. The Journal of Bone and Joint Surgery. American Volume, 62, 1039–1058. Faulkner K.G., Gluer C.C., Majumdar S., Lang P., Engelke
K., Genant H.K. (1991): Noninvasive measurements of bone mass, structure, and strength: current methods and experimental techniques. AJR. American Journal of Roentgenology, 157, 1229–1237.
Finkemeier C.G. (2002): Bone-grafting and bone-graft substitutes. The Journal of Bone and Joint Surgery. American Volume, 84-A, 454–464.
Finsen V., Haave O. (1987): Changes in bone-mass after tibial shaft fracture. Acta Orthopaedica Scandinavica,
Freeman L.M., Kehayias J.J., Roubenoff R. (1996): Use of dual-energy x-ray absorptiometry (DEXA) to meas-ure lean body mass, body fat, and bone mineral content (BMC) in dogs and cats. Journal of Veterinary Internal Medicine, 10, 99–100.
Grampp S., Jergas M., Gluer C.C., Lang P., Brastow P., Genant, H.K. (1993): Radiologic diagnosis of oste-oporosis. Current methods and perspectives. Radio-logic Clinics of North America, 31, 1133–1145. Grier S.J., Turner A.S., Alvis M.R. (1996): The use of
dual-energy x-ray absorptiometry in animals. Inves-tigative Radiology, 31, 50–62.
Haddad F.S., Duncan C.P. (2003): Cortical onlay allograft struts in the treatment of periprosthetic femoral frac-tures. Instructional Course Lectures, 52, 291–300. Horowitz M.C., Friedlaender G.E. (1987): Immunologic
aspects of bone transplantation. A rationale for future
studies. The Orthopedic Clinics of North America, 18, 227–233.
Jain R., Podworny N., Hearn T., Anderson G.I., Sche-mitsch E.H. (1997): Effect of stainless steel and tita-nium low-contact dynamic compression plate application on the vascularity and mechanical proper-ties of cortical bone after fracture. Journal of Ortho-paedic Trauma, 11, 490–495.
Kreuz F.P., Hyatt G.W., Turner T.C., Bassett A.L. (1951): The preservation and clinical use of freeze-dried bone. The Journal of Bone and Joint Surgery. American Vol-ume, 33-A, 863–872.
Lauten S.D., Cox N.R., Brawner W.R., Baker H.J. (2001): Use of dual energy x-ray absorptiometry for noninva-sive body composition measurements in clinically normal dogs. American Journal of Veterinary Re-search, 62, 1295–1301.
Malinin T., Latta L.L., Wagner J.L., Brown M.D. (1984): Healing of fractures with freeze-dried cortical bone plates. Comparison with compression plating. Clinical Orthopaedics and Related Research, 281–286. Millis D.L., Wilkens B.E., Daniel G.B., Hubner K.,
Math-ews A., Buonomo F.C., Patell K.R., Weigel J.P. (1998): Radiographic, densitometric, and biomechanical ef-fects of recombinant canine somatotropin in an un-stable ostectomy gap model of bone healing in dogs. Veterinary Surgery,27, 85–93.
Moyen B.J., Lahey P.J., Weinberg E.H., Harris W.H. (1978): Effects on intact femora of dogs of the applica-tion and removal of metal plates. A metabolic and structural study comparing stiffer and more flexible plates. The Journal of Bone and Joint Surgery. Amer-ican Volume,60, 940–947.
Perren S.M., Cordey J., Rahn B.A., Gautier E., Schneider E. (1988): Early temporary porosis of bone induced by internal fixation implants. A reaction to necrosis, not to stress protection? Clinical Orthopaedics and Re-lated Research, 139–151.
Schneider S., Breit S.M., Grampp S., Kunzel W., Lie-segang A., Mayrhofer E., Zentek J. (2004): Comparative assessment of bone mineral measurements obtained by use of dual-energy x-ray absorptiometry, peripheral quantitative computed tomography, and chemical-physical analyses in femurs of juvenile and adult dogs. American Journal of Veterinary Research, 65, 891– 900.
Sinibaldi K.R. (1989): Evaluation of full cortical allografts in 25 dogs. Journal of the American Veterinary Med-ical Association, 194, 1570–1577.
compression. The Journal of Bone and Joint Surgery. American Volume, 60, 516–522.
Theodorou D.J., Theodorou S.J. (2002): Dual-energy X-ray absorptiometry in clinical practice: Application and interpretation of scans beyond the numbers. Clinical Imaging, 26, 43–49.
Uhthoff H.K., Finnegan M. (1983): The effects of metal plates on post-traumatic remodelling and bone mass. The Journal of Bone and Joint Surgery. British Volume, 65, 66–71.
Vajaradul Y. (2000): Bangkok biomaterial center: 15 years experience in tissue banking. Cell Tissue Bank, 1, 229–239.
Wilson D., Frei H., Masri B.A., Oxland T.R., Duncan C.P. (2005): A biomechanical study comparing cortical on-lay allograft struts and plates in the treatment of periprosthetic femoral fractures. Clinical Biomechan-ics (Bristol, Avon), 20, 70–76.
Woo S.L., Akeson W.H., Coutts R.D., Rutherford L., Doty D., Jemmott G.F., Amiel D. (1976): A comparison of cortical bone atrophy secondary to fixation with plates with large differences in bending stiffness. The Journal of Bone and Joint Surgery. American Volume,58, 190–195.
Zhou Z., Pei F., Cheng J., Tu C., Liu L. (2005a): An ex-perimental study of the effect of biomechanical envi-ronment on the incorporation of cortical bone plates allografts. Sheng Wu Yi Xue Gong Cheng Xue Za Zhi, 22, 476–480.
Zhou Z. K., Pei F. X., Cheng J. Q., Tu C. Q., Lian Y. Y., Li X. Q. (2005b): Use of cortical bone plates allografts for reconstruction of femoral fracture: an experimen-tal study in goats. Sichuan Da Xue Xue Bao Yi Xue Ban, 36, 880–884.
Received: 2008–09–01 Accepted after corrections: 2009–04–08
Dr. Nam-Soo Kim, Associate Professor, Department of Surgery, College of Veterinary Medicine and Deputy Vice President for Academic Affairs, Chonbuk National University, Jeonju 561-756, Republic of Korea